An essential issue in the development of materials presenting an accurately functionalized surface is to achieve control of layer structuring. Whereas the very popular method based on the spontaneous adsorption of alkanethiols on metal faces stability problems, the reductive electrografting of aryldiazonium salts yielding stable interface, struggles with the control of the formation and organization of monolayers. Here we report a general strategy for patterning surfaces using aryldiazonium surface chemistry. Calixtetra-diazonium cations generated in situ from the corresponding tetra-anilines were electrografted on gold and carbon substrates. The well-preorganized macrocyclic structure of the calixarene molecules allows the formation of densely packed monolayers. Through adequate decoration of the small rim of the calixarenes, functional molecules can then be introduced on the immobilized calixarene subunits, paving the way for an accurate spatial control of the chemical composition of a surface at molecular level.
Surface functionalization has attracted considerable interest in recent years, with the aim to design surfaces with tailored properties (such as wettability, corrosion resistance, adhesion, lubricant, biocompatibility) or with operating functions ('smart' surfaces bearing stimuli-responsive architectures)1,2,3,4. When developed for modifying electrode surfaces, it finds applications in molecular electronics,5 bioelectronics6,7, and in the development of charge transport devices8,9 or sensors10. Particularly crucial for sensor studies, the controlled grafting of monolayers allows the design of complex recognition interfaces and provides responses akin to molecular level over the associated transduction reactions11.
Three major issues for constructing such interfaces can thus be pointed out: control of the thickness and density of the deposited layer, which ideally, as a first step, requires the formation of a monolayer; spatial control of the connected functions and robustness versus temperature, solvents, ageing.
The most popular strategy for fabricating monolayers is the spontaneous two-dimensional adsorption of thiol derivatives, especially alkanethiols, onto coinage metal (Pt, Au, Ag, Cu) forming self-assembled monolayers (SAMs) (Fig. 1a)12. Although highly versatile, this strategy could present important limitations related to their lack of thermal and long-term stability, narrow electrochemical window and stochastic behaviour of the gold–thiolate bond12,13,14. Besides, the spatial control of covalently bound functions is particularly difficult to achieve. Indeed, direct self-assembly of alkylthiols covalently connected at their extremity to functional objects generally leads to 'bouquet'-like repartition of the objects on the surface, with empty spaces in between (Fig. 1b)12. Dilution strategies with unfunctionalized alkylthiols allowing strong packing of the alkyl chain at the surface and simultaneous connection of large functional objects at the surface often lead to small 'islands of objects', not to regular distribution at the surface12,15,16,17,18,19. An alternative strategy for connecting organic moieties onto electrodes is the reductive grafting of aryldiazonium salts that yields covalent attachment of phenyl derivatives onto the surface. Electrografting in particular has gained tremendous interest over the last decade and is now a well-recognized method for surface functionalization20,21,22,23,24. Contrary to alkylthiol SAMs, the organic layers obtained from this method are generally highly stable, being strongly resistant to heat, chemical degradation and ultrasonication20,25. Furthermore, the method is easy to process and fast (deposition time on the order of 10 s instead of 10–18 h for well-organized thiol-Au SAMs) and can be applied to a wide range of materials: carbon (graphite, glassy carbon (GC), nanotubes, diamond), metals (Fe, Co, Ni, Cu, Zn, Pt, Au), semiconductor (SiH, SiO2, SiOC...), indium tin oxide and even organic polymers and dyes22. In spite of all these desirable properties, this strategy suffers from a major disadvantage, which is the poor control of layers thickness and regularity. Indeed, the reactive aryl radicals that are transiently produced attack not only the electrode surface but also already-grafted aryl layers, generally yielding multilayers and 'cauliflower'-like surfaces (Fig. 1c). This may result in the loss or decrease of efficiency of desirable properties, as observed for instance for the inferior charge transport properties of ferrocenyl redox moieties bound to such polyaryl layers26.
Although the diazonium grafting could be empirically controlled to some extent through the appropriate choice of experimental conditions (nature of solvent, aryldiazonium salt concentration, electrolysis time and applied potential), an ultrathin and homogeneous coating is generally difficult to obtain, thus limiting the capability of the method in designing complex surface patterning. Introduction of sterically encumbered substituents on the aryl rings has been successfully used to prevent the uncontrolled polymerization process, thus allowing the formation of a near monolayer27. However, an undesirable counterback is the chemical inertness of these molecules, which precludes further functionalization. To remedy this problem, aryldiazonium salts bearing a pendant function masked by a protecting group exhibiting steric hinderance28,29,30,31 and electronic shielding29 properties have been used (Fig. 1d). After removal of the protecting group, a postfunctionalization step allows for the attachment of functional molecules onto the newly activated monolayer. However, because of the leftover void spaces between two adjacent grafted aryl molecules after the deprotection step, this two-step strategy could be disadvantageous when the direct formation of compact, pinhole-free layers is desired. A very recent article describes a more straightforward one-step strategy based on the reductive electrografting of a benzene(p-bisdiazonium) salt, leaving a pendant diazonium protecting group for further chemical coupling32. However, this route suffers from a lack of long-term stability of the diazonium-terminated layers.
Here, we propose a different strategy based on surface pavement with versatile platforms that exhibit preorganization properties. This original concept uses rigid tetrapodant calixarenes33 as building blocks to form robust, closely packed and stable monolayers that can be postfunctionalized. Immobilization of calixarenes onto a surface by self-assembly techniques34 is classically achieved by anchoring the small rim of the calixarenes onto the substrate through their phenol or thiophenol functions. In contrast, our strategy relies on the large rim grafting of calixarenes, thanks to the diazonium coupling route, whereas the small rim is used for the introduction of spatially controlled postfunctionalizable groups. Adequate decorations of the small rim with appending arms make it possible to direct the introduction of functional molecules with a fine spatial control imposed by the geometry of the small rim, especially when two (or more) molecules are linked to the same calixarene. Close packing of the calix molecules and chemical control of the grafting process are ensured by the constrained cone conformation of the macrocycle that orients all four diazonium groups in the same direction and prevents polymerization of the transiently produced aryl radicals, thanks to the methylene bridges at the ortho-positions of the phenoxy substituents. It is noteworthy to mention that the preparation and the reductive grafting of calix[n]arenes fully substituted at the large rim by diazonium groups have never been reported.
Synthesis and grafting procedures of calixtetra-anilines
ptBu-calixarene was first O-alkylated by four alkyl or acyl groups following classical procedures. This allows to constrain the macrocycle in a cone conformation and to introduce at the small rim a carboxylic function that can easily be postfunctionalized. A sequence of ipso-nitration–reduction then yielded compounds 1–4 displayed in Fig. 2 (see the Supplementary Methods)35. Non-postfunctionalizable calixtetra-anilines 1 and 2 were first employed as model compounds for the surface modification and characterization, whereas compounds 3 and 4 were used to explore the postfunctionalization feasibility.
The grafting procedure was similarly conducted whatever the calixtetra-aniline or the nature of substrate used. The corresponding diazonium salts 1–4 were prepared in situ in 0.5 M aqueous HCl in the presence of NaNO2 (4 eq.)36. Gold, pyrolized photoresist film (PPF) or glassy carbon (GC) (disk electrodes) substrates were functionalized through the reduction of the in situ generated diazonium cations from calixtetra-anilines 1–4 either by six voltammetric cycles or by applying a constant potential. Figure 3a shows a typical cyclic voltammogram for the electrografting of 1 on a GC electrode taken as an example. It exhibits the characteristic behaviour of the reductive electrografting of aryldiazonium salts37. The potential was swept between +0.6 V and −0.6 V versus saturated calomel electrode (SCE). On the initial potential cycle, a broad irreversible peak located at about −0.25 V versus SCE was observed then, a dramatic decrease of current intensity was recorded upon the following cycles. The peak stems from the reduction of diazonium cations into phenyl radicals that subsequently react at the electrode surface, forming a covalently linked blocking layer at the electrode interface. Alternatively, the reduction of the in situ generated diazonium cations was performed by applying a constant potential at –0.5 V versus SCE for 5 min.
Characterization of the modified surfaces
After copious rinsing with a series of solvents (water, ethanol, dichloromethane, toluene) and drying under a stream of argon, the grafted layers were characterized by analysing their blocking properties toward the electrochemical response of redox probes such as Fe(CN)63−/4− (Supplementary Fig. S1), Ru(NH3)63+/2+ and dopamine.
Figure 3b–d shows typical voltammograms obtained with Ru(NH3)63+/2+ and dopamine from a GC electrode before and after electroreduction of the in situ generated diazonium cations from 2 or 4. As compared with the reversible redox processes at the bare electrode, a complete inhibition of the electrochemical response of the grafted surface was evidenced for all the redox probes. This indicates that an organic layer was formed at the electrode surface, and that this layer acts as a barrier for redox processes. Particularly informative regarding the compactness of the layer is the behaviour of dopamine. Oxidation of dopamine to the corresponding o-quinone has been demonstrated to require adsorption onto the GC electrode surface for exhibiting fast charge transfer kinetics and it was established that the coverage of the electrode surface with a dense monolayer is enough to inhibit the oxidation of dopamine38. Thus, observation of an electrochemical activity implies that the molecular probe could reach the carbon substrate that makes dopamine oxidation a specific test for detecting pinholes38,39. In our case, we observed the complete inhibition of the dopamine redox activity after the grafting of calixarenes 2 and 4 layers. This observation demonstrates that the possible pinholes/defects/empty spaces within the grafted layers have size smaller than that of dopamine.
To further characterize the grafted organic layer, contact angles of gold-modified substrates were measured using the sessile drop method (Fig. 4). The static contact angle with water was found to be 78±3° for the surface modified with 1 and 89±2° for the surface modified with 2, in comparison with the value of 62±2° for a bare gold surface.
These data indicate that hydrophobic films were formed on the gold surfaces due to the immobilization of the calixarenes. The larger contact angle for the surface modified with 2 is fully consistent with the stronger hydrophobic nature of the calixarene 2 as compared with 1. Remarkably, wetting studies for SAMs on gold formed with thio-calixarenes yielded similar contact angle values40,41.
X-ray photoelectron spectroscopy (XPS) analyses were performed on both PPF and gold substrates modified by the CF3-containing calixtetra-aniline 2, the CF3 groups providing a convenient chemical tag for XPS studies. The survey spectra showed main peaks corresponding to the elemental species C, N and O, whereas peaks due to Au were observed on gold substrates (Supplementary Fig. S2). In the case of gold substrates, an overall attenuation of the Au photoelectron peaks and a significant increase in the C1s and O1s peak heights, compared with the bare substrate, confirmed the coating of the gold substrate by an organic layer. A characteristic peak of the F1s photoelectrons appeared at 688.5 eV after surface functionalization by the calixarene 2. The presence of the CF3 group was further confirmed by the emergence of a new component at 293 eV in the C1s core level spectrum (Fig. 5). The C1s core level showed a main peak centred at 285 eV assigned to the aromatic carbons of the calixarene phenyl groups (and to the carbon atoms of the substrate when analysing the PPF substrates). A component at 286.2 eV was also evidenced, which corresponds to the C–O environment present in the calixarene frame. The small components at the high binding energy side (at ~287.3 and 289 eV) accounts for oxidized carbon from contamination species already detected on the bare substrates.
The absence of a N1s peak attributed to –N2+ (at 403.8 eV) indicates a complete transformation of the diazonium cations, whereas the very low intensity signal at 400 eV reveals the formation of a very small proportion of azo groups (–N=N–) derived from the diazonium salts as already reported in the literature36,42,43,44,45,46.
Atomic force microscopy (AFM) analysis was performed by using preferentially PPF substrates because of their low surface roughness in comparison with GC or gold substrates employed in this work. PPF plates grafted with the reduction of diazonium cations issued from 1 or 2 showed surface structures almost identical and of same sizes as the bare PPF, indicating a uniform deposit on the whole surface (Fig. 6). The surface roughness increased only slightly upon the electrografting of the calixarenes (root-mean-square roughness, r.m.s.<1 nm) as compared with a bare PPF substrate (r.m.s.<0.8 nm)47. These observations fall in line with the formation of very thin layers. Remarkably, the surface roughness was not affected by electrolysis time (30 s, 1 min, 5 min, 10 min) employed for the electrografting of the in situ generated diazonium cations, suggesting that the system is self-inhibiting.
AFM technique was further used for estimating the thicknesses of the organic layers. The AFM tip was used in contact mode to scratch a rectangular area on the PPF functionalized samples by exercising a force sufficient to remove the organic part without damaging the PPF sample. Profiling depth measurements of the scratched area in an intermittent contact mode gave the average thickness of the layer, as described by Mc Creery and co-workers48. The thickness was thus estimated to be 1.3±0.1 nm (Fig. 6c). This result agrees well with the height of calixarenes 1 and 2 (c.a. 1.0 and 1.1 nm, respectively, estimated from MM2 energy minimizations with ChemBio3D software), and indicates that the electrografting of the corresponding diazonium cations led to the formation of monolayers. This result is further confirmed by ellipsometric measurements of gold substrates modified with calixarene 2. Thickness value of 1.09±0.20 nm was found, in very good agreement with the height of calixarene 2. Both techniques unambiguously demonstrate the formation of monolayers. From the strong blocking effect toward redox probe responses, namely regarding the answer of the monolayer towards dopamine, it can be further concluded that the formed monolayers are rather compact.
Taking account the formation of monolayers, XPS data could be used to give a reliable estimation of surface coverage for the non-electroactive calixarene 2. On gold samples, the average calixarene coverage α on the gold surface could be expressed from F1s and Au4f peak intensities related to calixarenes layers and the gold substrate, respectively49. The calculation (details provided in the Supplementary Methods) leads to a surface coverage α of the gold substrate by the calixarene 2 molecules of 79%. Calixarenes present an external diameter of 14 Å (large rim)50. Considering a hexagonal compact arrangement of disks (or spheres) of 14 Å diameter, the surface concentration for the closest packing of calixarenes corresponds to ΓCPML=9.8×10−11 mol cm−2 and the closest-packing monolayer covers 90.7% of the gold surface. It comes that the surface concentration of calixarene 2 onto gold substrate estimated from XPS data is equal to 8.5×10−11 mol cm−2 (0.5 calix nm−2).
All these results evidence the formation of a dense and compact monolayer of calixarenes.
Postfunctionalization of the modified surfaces
Having demonstrated the straightforward formation of monolayers from the electroreduction of diazonium cations derived from compounds 1 and 2, calixtetra-anilines 3 and 4 (Fig. 7) were then used to modify substrates as a proof-of-concept for postfunctionalization purposes. The presence of one (for 3) or four (for 4) appending carboxyl group(s) at the calixarenes small rim allows a further chemical coupling using acyl chloride activation. Accordingly, ferrocene moieties were covalently introduced through an amide bond formation with ferrocenemethylamine (FcCH2NH2) following a procedure previously described (Fig. 7)51.
After the chemical postfunctionalization, the modified substrates were thoroughly rinsed with CH2Cl2, then transferred to a pure CH2Cl2 + 0.2 M NBu4PF6 electrolyte solution. Well-defined oxidation and reduction peaks corresponding to the introduced ferrocene/ferrocenium couple were detected at c.a. 0.4 V versus SCE, as illustrated in Fig. 8. It was also observed that the current linearly increased with scan rate in the (0.05–10 V s−1) range as expected for surface-confined electroactive species.
For experiments using calixarene 3 (Fig. 8a), the surface density of attached ferrocene centres was derived from integration of the voltammetric peaks at low scan rates. This allowed an estimation of the surface coverage of calixarenes themselves onto the substrate since each calixarene frame bears one functionalizable carboxyl substituent. Because the postfunctionalization reaction may not take place with 100% yield, this value could be regarded as a lower estimate of the calixarenes surface concentration. Surface concentration was found to be Γ1=6.9±0.6×10−11 mol cm−2, corresponding to a density of 0.42 calix nm−2. This result is fully consistent with the surface concentration value estimated from XPS data and confirms the formation of rather densely packed monolayers, in line with the good blocking properties of the layers towards the electronic transfer. Note that the surface concentration here found is in good agreement with surface concentration reported for gold–thiols SAMs of calixarenes52,53, or compares favourably with the density reported for the covalent and rigid grafting of calixarenes onto silica surfaces54, the molecular footprint of the described calixarenes being similar to the calixarenes 1–4.
The surface concentration of electroactive ferrocene was similarly determined for experiments using the tetra-carboxylic acid decorated calixtetra-aniline 4. A surface concentration Γ2=1.6±0.4×10−10 mol cm−2 was calculated. This surface concentration is one third the value reported for the closest packing of ferrocene55 and corresponds to c.a. twice the Γ1 value. This result indicates that two ferrocenyl moieties could be attached onto each calixarene subunit. This allows the introduction of functional groups on the surface with a precise spatial control, which is imposed by the calixarene small rim geometry.
Calixtetra-anilines have been successfully electrografted to various substrates by generating in situ their corresponding diazonium cations. Thanks to its well-preorganized and unique 3D conic structure, the calixarene core prevents the formation of multilayers and leads to densely packed monolayers56. Characterization of the modified surfaces points out to an efficient packing of the calix molecules, probably ensured by the constrained cone conformation of the macrocycle that orients all four diazonium groups in the same direction. However, this does not necessarily imply that four aryl–substrate bonds are formed. This would depend on the availability of gold or carbon atoms sites and the possible degree of distortion of the calixarene molecule (Supplementary Fig. S3). The important point is that the calix grafts with its cone axis perpendicular to the surface, whatever the number of aryl–substrate bonds formed, and the thicknesses reported in this work are in good agreement with this point. Providing that the calixarene platforms possess chemically reactive appending arms at the small rim, this strategy allows for the straightforward preparation of versatile robust monolayers that can be directed at the spatially controlled introduction of functional entities. This approach can be made even more sophisticated by using calixarenes that exhibit two different anchoring termini on the same frame, thus opening new possibilities for the design of multicomponent films with a spatial control at the molecular level. Work is currently under way to implement this last approach.
The synthesis of the various calixarenes compounds and their characterization are described in the Supplementary Methods.
Surface modifications procedures
The reagents and solvents used for surface chemistry were of high purity grade (Sigma-Aldrich, SDS, Alfa Aesar). The GC substrates were home-made disk electrodes of 3 mm diameter, thoroughly polished (successively with 5 μm SiC paper (Struers), 1 μm DP–Nap paper (Struers) with 0.3 μm Al2O3 slurry (Struers)) and rinsed with ultrapure water, and absolute ethanol under sonication. Gold substrates (gold layer onto Si substrates) were purchased from Aldrich and thoroughly cleaned before surface functionalization (piranha solution). PPF samples were prepared according to previously published procedure57. Surface modification by electrochemical reduction of in situ generated diazonium cations was carried out in an ice bath. NaNO2 (4 eq.) was added to the aqueous electrolytic solution containing 5 mmol−1 calixtetra-aniline and 0.5 mol−1 HCl under stirring. After 5 min, the modification was achieved potentiostatically or by potential cycling between 0.6 and −0.6 V/SCE. After modification, the substrates were rinsed (sonication) with ultrapure water, abs EtOH, freshly distiled CH2Cl2 and toluene (high-performance liquid chromatography grade). The subsequent ferrocenyl postfunctionalization was carried out according to ref. 51.
Cyclic voltammograms were recorded with an Autolab electrochemical analyzer (PGSTAT 30 potentiostat/galvanostat from Eco Chemie B.V.) in a three-electrode setup with an SCE reference electrode and a platinum foil as counter electrode.
The surface coverage of electroactive ferrocene is obtained from Faraday's Law, Γ=Q/nFA where Q is the charge passed, n the number of exchanged electrons, F the Faraday constant and A the area of electrode. Q is obtained from the integration of the area under the voltammetric peaks at low scan rates using the integration function of the Origin software. Polynomial baselines can be solved and subtracted before the curve integration.
AFM microscopy analyses
AFM experiments used a Picoscan II microscope (Agilent) coupled to a pico-SCAN2500 controller. The images were acquired in acoustic mode using silicon nitride tips (resonance frequency c.a 350 kHz). Scratching technique was used to determine the thickness of the organic layer grafted on the PPF samples. Square-shaped scratches were obtained in contact mode with a force set-point voltage around 1 V. Several depth-profiles were measured for each scratched region. Height distributions were also investigated on images to confirm the depth-profiles measurements.
XPS photoelectron spectra were collected from modified GC and gold plates on a Thermo VG Scientific Escalab 250 system fitted with a monochromatic Al Kα X-ray source (hν=1486.6 eV, spot size=650 μm, power 15 kV×200 W). The pass energy was set at 150 and 40 eV for the survey and the narrow regions, respectively. Spectral calibration was determined by setting the main C1s component at 285 eV. The surface composition was estimated using the integrated peak areas and the corresponding Scofield sensitivity factors corrected for the analyzer transmission function.
Contact angle measurements
The static contact angles of 2 μl ultrapure water drops were measured on four different spots on the surface with an easy drop goniometer (Krüss). The contact angles were determined using a tangent 2 or circle fitting models.
Thicknesses of the layers on Au were measured with a mono wavelength ellipsometer Sentech SE400. The following values were taken for gold: ns=0.203, ks=3.431. These values were measured on clean surfaces before grafting and the layers thicknesses were determined from the same plates after modification, taking ns=1.5, ks=0 for the layer. Measurements reported are the average of ten data points across each substrate (two substrates were analysed).
How to cite this article: Mattiuzzi, A. et al. Electrografting of calixarenediazonium salts to form versatile robust platforms for spatially controlled surface functionalization. Nat. Commun. 3:1130 doi: 10.1038/ncomms2121(2012).
Simao, C. et al. A robust molecular platform for non-volatile memory devices with optical and magnetic responses. Nat. Chem. 3, 359–364 (2011).
Areephong, J., Browne, W. R., Katsonis, N. & Feringa, B. L. Photo- and electro-chromism of diarylethene modified ITO electrodes - towards molecular based read-write-erase information storage. Chem. Commun. 3930–3932 (2006).
Amatore, C., Genovese, D., Maisonhaute, E., Raouafi, N. & Schollhorn, B. Electrochemically driven release of picomole amounts of calcium ions with temporal and spatial resolution. Angewandte Chem. Int. Ed. 47, 5211–5214 (2008).
Lahann, J. et al. A reversibly switching surface. Science 299, 371–374 (2003).
Kim, B. S. et al. Temperature and length dependence of charge transport in redox-active molecular wires incorporating ruthenium(II) bis (σ-arylacetylide) complexes. J. Phys. Chem. C 111, 7521–7526 (2007).
Willner, I. Biomaterials for sensors,fuel cells, and circuitry. Science 298, 2407–2408 (2002).
Choi, H. J., Kim, N. H., Chung, B. H. & Seong, G. H. Micropatterning of biomolecules on glass surfaces modified with various functional groups using photoactivatable biotin. Anal. Biochem. 347, 60–66 (2005).
Adams, D. M. et al. Charge Transfer on the nanoscale: current status,. J. Phys. Chem. B 107, 6668–6697 (2003).
Finklea, H. O. Electrochemistry of organized monolayers of thiols and related molecules on electrodes. in Electroanalytical chemistry, Vol 19 (eds Bard A.J. and Rubinstein) 109–337 (Marcel Dekker, Inc. New York, 1996).
Gooding, J. J. Advances in interfacial design for electrochemical biosensors and sensors: aryl diazonium salts for modifying carbon and metal electrodes. Electroanalysis 20, 573–582 (2008).
Gooding, J. J. & Ciampi, S. The molecular level modification of surfaces : from self-assembled monolayers to complex molecular assemblies. Chem. Soc. Rev. 40, 2704–2718 (2011).
Love, C. J., Estroff, L. A., Kriebel, J. K., Nuzzo, R. G. & Whitesides, G. M. Self-assembeld monolayers of thiolates on metal as a form of nanotechnology. Chem. Rev. 105, 1103–1169 (2005).
Vericat, C., Vela, M. E., Benitez, G., Carro, P. & Salvarezza, R. C. Self-assembled monolayers of thiols and dithiols on gold : new challenges for a well-known system. Chem. Soc. Rev. 39, 1805–1834 (2010).
Kind, M. & Wöll, C. Organic surfaces exposed by self-assembled organothiol monolayers: preparation, characterization, and application. Progr. Surf. Sci. 84, 230–278 (2009).
Sullivan, T. P. & Huck, W. T. S. Reactions on monolayers: organic synthesis in two dimensions. Eur. J. Org. Chem. 17–23 (2003).
Bain, C. D. & Whitesides, G. M. Formation of monolayers by the coadsorption of thiols on gold: variation in the length of the alkylchain. J. Am. Chem. Soc. 111, 7164–7175 (1989).
Folkers, J. P., Laibinis, P. E. & Whitesides, G. M. Self-assembled monolayers of alkanethiols on gold: comparisons of monolayers containing mixture of short- and long-chain constituents with CH3 and CH2OH terminal groups. Langmuir 8, 1330–1341 (1992).
Stranick, S. J., Parikh, A. N., Tao, Y. T., Allara, D. L. & Weiss, P. S. Phase separation of mixed-composition self assembled monolayers into nanometer scale molecular domains. J. Phys. Chem. 98, 7636–7646 (1994).
Tamada, K., Akiyama, H., Wei, T. X. & Kim, S. A. Photoisomerization reaction of unsymmetrical azobenzene disulfide self-assembled monolayers: modification of azobenzene dyes to improve thermal endurance for photoreaction. Langmuir 19, 2306–2312 (2003).
Downard, A. J. Electrochemically assisted covalent modification of carbon electrodes. Electroanalysis. 11, 1085–1096 (2000).
Pinson, J. & Podvorica, F. Attachment of organic layers to conductive or semiconductive surfaces by reduction of diazonium salts. Chem. Soc. Rev. 34, 429–439 (2005).
Pinson, J. & Bélanger, D. Electrografting: a powerful method for surface modification. Chem. Soc. Rev. 40, 3995–4048 (2011).
Mahouche-Chergui, S., Gam-Derouich, S., Mangeney, C. & Chehimi, M. H. Aryl diazonium salts: a new class of coupling agent for bonding polymers, biomacromolecules and nanoparticles to surfaces. Chem. Soc. Rev. 40, 4143–4166 (2011).
Aryl Diazonium Salts. New Coupling Agents in Polymer and Surface Science (ed. Chehimi, M.M.), (Wiley-VCH, Weinheim, 2012).
Gui, A. L. et al. A comparative study of modifying gold and carbon electrode with 4-sulfophenyl diazonium salt. Electroanalysis 22, 1283–1289 (2010).
Zigah, D., Noel, J. M., Lagrost, C. & Hapiot, P. Charge transfer electroactive species immobilized on carbon surfaces by aryl diazonium reduction. SECM investigations. J. Phys. Chem. C 114, 3075–3081 (2010).
Combellas, C., Kanoufi, F., Pinson, J. & Podvorica, F. I. Sterically hindered diazonium salts for the grafting of a monolayer on metals. J. Am. Chem. Soc. 130, 8576–8577 (2008).
Leroux, Y. R., Fei, H., Noel, J.- M., Roux, C. & Hapiot, P. Efficient covalent modification of a carbon Surface: Use of a silyl protecting group to form an active monolayer. J. Am. Chem. Soc. 132, 14039–14041 (2010).
Malmos, K. et al. Using a hydrazone-protected benzenediazonium salt to introduce a near-monolayer of benzaldehyde on glassy carbon surfaces. J. Am. Chem. Soc. 131, 4928–4938 (2009).
Nielsen, L. T. et al. Electrochemical approach for constructing a monolayer of thiophenolates from grafted multilayers of diaryl disulfides. J. Am. Chem. Soc. 129, 1888–1889 (2007).
Peng, Z., Holm, A. H., Nielsen, L. T., Pedersen, S. U. & Daasberg, K. Covalent sidewall functionalization of carbon nanotubes by a “formation-degradation” approach. Chem. Mater. 20, 6068–6075 (2008).
Marshall, N. & Locklin, J. Reductive electrografting of benzene (p-bisdiazonium hexafluorophosphate): a simple and effective protocol for creating diazonium-functionalized thin films. Langmuir 27, 13367–13373 (2011).
Gutsche, C. D. in Calixarenes Revisited, Monographs in Supramolecular Chemistry (ed. Stoddart, J.F.), (The Royal Society of Chemistry, Cambridge, 1998).
Kim, H. J., Lee, M. H., Mutihac, L., Vicens, J. & Kim, J. S. Host-guest sensing by calixarenes on the surface. Chem. Soc. Rev. 41, 1173–1190 (2012).
Sansone, F., Chierici, E., Casnati, A. & Ungaro, R. Thiourea-linked upper rim calixarene neoglycoconjugates: synthesis, conformations and binding properties. Org. Biomol. Chem. 1, 1802–1809 (2003).
Baranton, S. & Bélanger, D. Electrochemical derivatization of carbon surface by reduction of in situ generated diazonium cations. J. Phys. Chem. B 109, 24401–24410 (2005).
Delamar, M., Hitmi, R., Pinson, J. & Savéant, J. -M. Covalent modification of carbon surfaces by grafting of functionalized aryl radicals produced from electrochemical reduction of diazonium salts. J. Am. Chem. Soc. 114, 5883–5884 (1992).
DuVall, S. H. & McCreery, R. L. Control of catechol and hydroquinone electron-transfer kinetics on native and modified glassy carbon electrodes. Anal. Chem. 71, 4594–4602 (1999).
DuVall, S. H. & McCreery, R. L. Self-catalysis by catechols and Quinones during heterogeneous electron transfer at carbon electrodes. J. Am. Chem. Soc. 122, 6759–6764 (2000).
Cygan, M. T. et al. Calixarene monolayers as quartz crystal microbalance sensing element in aqueous solution. Anal. Chem. 71, 142–148 (1999).
Zhang, S., Song, F. & Echegoyen, L. Synthesis, self-assembled monolayers and alkaline earth metal ion recognition of p-tert-butylcalixarene derivatives. Eur. J. Org. Chem. 2936–2943 (2004).
Toupin, M. & Bélanger, D. Thermal stability study of aryl modified carbon black in situ generated diazonium salt. J. Phys. Chem. C 111, 5394–5401 (2007).
Saby, C., Ortiz, B., Champagne, G. Y. & Bélanger, D. Electrochemical modification of glassy carbon electrode using aromatic diazonium salt. 1. Blocking effect of 4-nitrophenyl and 4-carboxyphenyl groups. Langmuir 13, 6805–6813 (1997).
Lyskawa, J. & Bélanger, D. Direct modification of a gold electrode with aminophenyl groups by electrochemical reduction of in situ generated aminophenyl monodiazonium cations. Chem. Mater. 18, 4755–4763 (2006).
Hurley, B. L. & McCreery, R. L. Covalent bonding of organic molecules to Cu and Al alloy 2024 T3 surfaces via diazonium ion reduction. J. Electrochem. Soc. 151, B252–B259 (2004).
Doppelt, P., Hallais, G., Pinson, J., Podvorica, F. & Verneyre, S. Surface modification of conducting substrates. Existence of azo bonds in the structure of organic layers obtained from diazonium salts. Chem. Mater. 19, 4570–4575 (2007).
Ranganathan, S. & McCreery, R. L. Electroanalytical performance of carbon films with near-atomic flatness. Anal. Chem. 73, 893–900 (2001).
Anariba, F., DuVall, S. H. & McCreery, R. L. Mono- and multilayer formation by diazonium reduction on carbon surfaces monitored with atomic force microscopy 'scratching'. Anal. Chem. 75, 3837–3844 (2003).
Dahoumane, S. A et al. Protein-functionalized hairy diamond nanoparticles. Langmuir 25, 9633–9638 (2009).
Kim, J. -H., Kim, Y. -G., Lee, K. -H., Kang, S. -W. & Koh, K. -N. Size selective molecular recognition of calixarenes in Langmuir-Blodgett monolayers. Synth. Met. 117, 145–148 (2001).
Noel, J. -M., et al. Flexible strategy for immobilizing redox-active compounds using in situ generation of diazonium salts. Investigation of the blocking and catalytic properties of the layers. Langmuir 25, 12742–12749 (2009).
Chen, H. et al. Comparative study of protein immobilization properties on calixarenes monolayers. Sensors 7, 1091–1107 (2007).
Cormode, D. P., Evans, A. J., Davis, J. J. & Beer, P. D. Amplification of anion sensing by disulfide functionalized ferrocene and ferrocene-calixarene receptors adsorbed onto gold surfaces. Dalton Trans. 39, 6532–6541 (2010).
Notestein, J. M., Katz, A. & Iglesia, E. Energetics of small molecule and water complexation in hydrophobic calixarene cavities. Langmuir 22, 4004–4014 (2006).
Seo, K., Jeon, I. C. & Yoo, D. J. Electrochemical characteristics of ferrocenecarboxylate-coupled aminoundecylthiol self-assembled monolayers. Langmuir 20, 4147–4154 (2004).
Mattiuzzi, A., Jabin, I., Reinaud, O., Hapiot, P. & Lagrost, C. European patent EP 12164038 (2012).
Brooksby, P. A. & Downard, A. J. Electrochemical and atomic force microscopy study of carbon surface modification via diazonium reduction in aqueous and acetonitrile solutions. Langmuir 20, 5038–5045 (2004).
This work was supported by the Agence Nationale de la Recherche (ANR10-BLAN-714 Cavity-zyme(Cu) project) and by the FNRS (A.M. PhD grant). We thank Pr. A.J. Downard (University of Canterbury, N.Z.) for fruitful discussions and advices concerning PPF samples.
The authors declare no competing financial interests.
About this article
Cite this article
Mattiuzzi, A., Jabin, I., Mangeney, C. et al. Electrografting of calixarenediazonium salts to form versatile robust platforms for spatially controlled surface functionalization. Nat Commun 3, 1130 (2012). https://doi.org/10.1038/ncomms2121
The electro-oxidation of primary alcohols via a coral-shaped cobalt metal–organic framework modified graphite electrode in neutral media
Scientific Reports (2022)
Scientific Reports (2019)
Scientific Reports (2016)